# 1.07 Quantum Dots: quantum dots, sometimes termed as electrostatic quantum dots, can be controlled...

date post

26-Jun-2020Category

## Documents

view

4download

0

Embed Size (px)

### Transcript of 1.07 Quantum Dots: quantum dots, sometimes termed as electrostatic quantum dots, can be controlled...

1.07 Quantum Dots: Theory N Vukmirović and L-W Wang, Lawrence Berkeley National Laboratory, Berkeley, CA, USA

ª 2011 Elsevier B.V. All rights reserved.

1.07.1 Introduction

1891.07.2 Single-Particle Methods

1901.07.2.1 Density Functional Theory

1911.07.2.2 Empirical Pseudopotential Method

1931.07.2.3 Tight-Binding Methods

1941.07.2.4 k ? p Method

1951.07.2.5 The Effect of Strain

1981.07.3 Many-Body Approaches

2011.07.3.1 Time-Dependent DFT

2011.07.3.2 Configuration Interaction Method

2021.07.3.3 GW and BSE Approach

2031.07.3.4 Quantum Monte Carlo Methods

2041.07.4 Application to Different Physical Effects: Some Examples

2051.07.4.1 Electron and Hole Wave Functions

2051.07.4.2 Intraband Optical Processes in Embedded Quantum Dots

2061.07.4.3 Size Dependence of the Band Gap in Colloidal Quantum Dots

2081.07.4.4 Excitons

2091.07.4.5 Auger Effects

2101.07.4.6 Electron–Phonon Interaction

2121.07.5 Conclusions

213References

2131.07.1 Introduction

Since the early 1980s, remarkable progress in technology

has been made, enabling the production of nanometer-

sized semiconductor structures. This is the length scale

where the laws of quantum mechanics rule and a range

of new physical effects are manifested. Fundamental

laws of physics can be tested on the one hand, while on the other hand many possible applications are rapidly

emerging for nanometer-sized semiconductors.. The ultimate nanostructure where carriers are

confined in all the three spatial dimensions is called

a quantum dot. In the last 15 years, quantum dots

have been produced in several different ways in a

broad range of semiconductor material systems. The properties of quantum dots and their possible appli-

cations are largely dependent on the method they

have been obtained with, which can, therefore, be

used as a criterion for classification of different

types of quantum dots: Electrostatic quantum dots. One can fabricate quan-

tum dots by restricting the two-dimensional (2D) electron gas in a semiconductor heterostructure

laterally by electrostatic gates or vertically by etch- ing techniques [1,2]. The properties of this type of quantum dots, sometimes termed as electrostatic quantum dots, can be controlled by changing the applied potential at gates, the choice of the geometry of gates, or external magnetic field. The typical size of these dots is of the order of 100 nm.

Self-assembled quantum dots. Self-assembled quantum dots are obtained in heteroepitaxial systems with dif- ferent lattice constants. During the growth of a layer of one material on top of another, the formation of nanoscale islands takes place [3], if the width of the layer (the so-called wetting layer) is larger than a certain critical thickness. This growth mode is called Stranski–Krastanov mode. The most common experi- mental techniques of the epitaxial nanostructure growth are molecular beam epitaxy (MBE) and meta- lorganic chemical vapor deposition (MOCVD) [4,5]. Since the quantum dot material is embedded in another material, we refer to these dots also as embedded quantum dots. Self-assembled quantum dots typically have lateral dimensions of the order of 15–30 nm and height of the order 3–7 nm.

189

190 Quantum Dots: Theory

Colloidal quantum dots. A very different approach to obtain quantum dots is to synthesize single crystals

of the size of a few nanometers through chemical

methods. The dots obtained in this way are called

nanocrystals or colloidal quantum dots [6]. Their

size and shape can be controlled by the duration,

temperature, and ligand molecules used in the synth-

esis [7]. Colloidal quantum dots are typically of

spherical shape. They are often smaller than

embedded quantum dots with the diameter some-

times as low as 2–4 nm. Quantum dots have enabled the study of many

fundamental physical effects. Electrostatic quantum

dots can be controllably charged with a desired

number of electrons and therefore the whole periodic

system [8] of artificial atoms created, providing a

wealth of data from which an additional insight into

the many-body physics of fermion systems could be

obtained [1]. Single-electron transport and Coulomb

blockade effects on the one hand, and the regime of

Kondo physics on the other hand, have been investi-

gated [9,10]. One of the most exciting aspects of quantum dot

research is certainly the prospect of using the state of

the dot (spin state, exciton, or charged exciton) as a

qubit in quantum information processing. Coherent

control of an exciton state in a single dot selected

from an ensemble of self-assembled quantum dots as

well as the manipulation of the spin state in electro-

static quantum dots [12,13] have been achieved [11].

The theoretical and experimental progress in the

field of spin-related phenomena in quantum dots

has been reviewed in Refs. [1 and 14]. These results

appear promising, although the control of a larger

number of quantum dot qubits is not feasible yet,

mainly due to difficulty in controlling qubit–qubit

interactions. The practical applications of quantum dots

certainly do not lag behind these exciting areas of

fundamental science with quantum dots. For exam-

ple, colloidal quantum dots have found several

cutting-edge applications such as fluorescent biolo-

gical labels [15], highly efficient photovoltaic solar

cells [16], and nanocrystal-based light-emitting

diodes [1]. Self-assembled quantum dots find the

main application as optoelectronic devices – lasers

[17], optical amplifiers [18], single-photon sources

[19,20], and photodetectors [21,22,23]. This chapter focuses on theoretical methods used

for calculation of physical properties of self-

assembled and colloidal quantum dots.

1.07.2 Single-Particle Methods

While quantum dots seem to be small and simple

objects, a look at their structure from the atomistic

side reveals their high complexity. Bearing in mind

that the lattice constants of the underlying semicon-

ductor materials are typically of the order of 0.5 nm,

one can estimate that a single self-assembled quan-

tum dot contains �106 nuclei and even a larger number of electrons interacting among each other

with long-range Coulomb forces. Even the smallest

colloidal quantum dots contain thousands of atoms. This clearly indicates that direct solution of the

many-body quantum dot Hamiltonian is not a feasi-

ble approach and that smart and efficient methods

need to be developed. Here, methods that reduce the

problem to an effective single-particle equation are

reviewed. More than two decades ago, Brus introduced

[24–25] a simple effective mass method to calculate

ionization energies, electron affinities, and optical

transition energies in semiconductor nanocrystals.

Within Brus’s model, the single-particle (electron or

hole) energies E and wave functions (r) satisfy the Schrödinger’s equation given as

– 1

2m� r2 þ PðrÞ

� � ðrÞ ¼ E ðrÞ ð1Þ

where m� is the electron or hole effective mass. The system of atomic units where the reduced Planck’s constant h�, the electron mass m0, and the electron charge c are all equal to 1 was used in equation 1 and will be used in what follows. For simplicity, equation 1 assumes that the particle must be confined within the dot, that is, that the potential outside the dot is infinite. This simplifying assumption can be easily relaxed by adding a more realistic confining potential Vconf (r).

P(r) in equation 1 is the additional potential caused by the presence of the surface of the quantum dot. It

has a certain analogy with electrostatic image poten-

tials in the case when a charge is near the surface of the

metal or the interface between two dielectrics. It can

be obtained by calculating the interaction energy

between a bare electron and its induced screening

potential. The extra interaction energy of an electron

at r inside the quantum dot compared to the corre-

sponding value in bulk is then P(r). To model the two-particle excitations (such

as electronþ hole¼ exciton), Brus introduced an

Quantum Dots: Theory 191

electrostatic interaction energy term among these particles as

V ðr1;r2Þ ¼ � e2

" r1–r2j j � PM r1;r2ð ÞþP r1ð ÞþP r2ð Þ ð2Þ

where " is the dielectric constant, PM corresponds to the interaction of the charge of one particle with surface-induced polarization potential of the other particle, while the P-terms describe the interaction of the charge of one particle with its own surface- induced polarization potential, as previously described. The plus (minus) sign is for the two par- ticles of the same (opposite) charge. The effective exciton Hamiltonian is then given as

Hexciton ¼ – 1

2me r2e –

1

2mh r2h –

e2

� re – rhj j

– PMðre; rhÞ þ PðreÞ þ PðrhÞ ð3Þ

The solution of the eigenvalue problem of this Hamiltonian can be written down analytically as

E�. Eg

*View more*